LMucko/crystallography-open-database huggingface dataset:
Crystal structure of alpha-Mg2 P2 O7 and the mechanism of the phase transition beta-alpha-Mg2 P2 O7
Lukaszewicz, K.; Bulletin de l'Academie Polonaise des Sciences, Serie des Sciences Chimiques 15 (1967) 53–57; doi:

data_1542047
_publ_section_title
;
 Crystal structure of alpha-Mg2 P2 O7 and the mechanism of the phase
 transition beta-alpha-Mg2 P2 O7
;
_journal_name_full
;
Bulletin de l'Academie Polonaise des Sciences, Serie des Sciences Chimiques
;
_journal_page_first              53
_journal_page_last               57
_journal_volume                  15
_journal_year                    1967
_chemical_formula_sum            'Mg2 O7 P2'
_chemical_name_systematic        'Mg2 (P2 O7)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc (1/2*x,y,-1/2*x+z)'
_symmetry_space_group_name_H-M   'P 1 21/c 1 (2*a+c,b,c)'
_cell_angle_alpha                90
_cell_angle_beta                 105.18
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   13.172
_cell_length_b                   8.29
_cell_length_c                   9.053
_cell_volume                     954.058
_citation_journal_id_ASTM        BAPCAQ
_cod_data_source_file            Lukaszewicz_BAPCAQ_1967_1723.cif
_cod_data_source_block           Mg2O7P2
_cod_original_cell_volume        954.0578
_cod_database_code               1542047
Die Kalium-Wolframbronzen und Natrium-Kalium-Wolframbronzen
Straumanis, M.E.; Ma, C.H.; Das Gupta, S.C.; Zeitschrift fuer Anorganische und Allgemeine Chemie 265 (1951) 209–219; doi:

data_1542048
_publ_section_title
;
 Die Kalium-Wolframbronzen und Natrium-Kalium-Wolframbronzen
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              209
_journal_page_last               219
_journal_volume                  265
_journal_year                    1951
_chemical_formula_sum            'Na0.11 O3 W'
_chemical_name_systematic        'Na0.11 (W O3)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8351
_cell_length_b                   3.8351
_cell_length_c                   3.8351
_cell_volume                     56.407
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Straumanis_ZAACAB_1951_881.cif
_cod_data_source_block           Na0.11O3W1
_cod_original_cell_volume        56.40662
_cod_original_formula_sum        'Na0.11 O3 W1'
_cod_database_code               1542048
Structure cristalline de l'acide nitrique anhydre.
Luzzati, V.; Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences (1884 - 1965) 229 (1949) 1349–1351; doi:

data_1542049
_publ_section_title
;
 Structure cristalline de l'acide nitrique anhydre.
;
_journal_name_full
;
Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences (1884 - 
1965)
;
_journal_page_first              1349
_journal_page_last               1351
_journal_volume                  229
_journal_year                    1949
_chemical_formula_sum            'H N O3'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   16.23
_cell_length_b                   8.57
_cell_length_c                   6.31
_cell_volume                     877.665
_citation_journal_id_ASTM        COREAF
_cod_data_source_file            Luzzati_COREAF_1949_81.cif
_cod_data_source_block           H1N1O3
_cod_depositor_comments
;
Fixing positions of O4 and O10 (removing the errorneous "-" sign from
the y coordinates) after consulting the Acta Cryst. paper (Luzzati,
V. (1951). Acta Cryst. 4, 120-131, DOI:10.1107/S0365110X51000404) that
seems to describe exactely the same structure. Now the NO2 geometry is
much more reasonable.

Saulius Gra\<zulis
2017-07-31
;
_cod_original_cell_volume        877.6648
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'H1 N1 O3'
_cod_database_code               1542049
Barium Cobalt Oxide of the Perowskite Type
Strauss, S.W.; Fankuchen, I.; Ward, R.; Journal of the American Chemical Society 73 (1951) 5084–5086; doi:

data_4124851
_publ_section_title
;
 Barium Cobalt Oxide of the Perowskite Type
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              5084
_journal_page_last               5086
_journal_volume                  73
_journal_year                    1951
_chemical_formula_sum            'Ba Co O2.23'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.072
_cell_length_b                   4.072
_cell_length_c                   4.072
_cell_volume                     67.519
_citation_journal_id_ASTM        JACSAT
_cod_data_source_file            Strauss_JACSAT_1951_995.cif
_cod_data_source_block           Ba1Co1O2.23
_cod_original_cell_volume        67.51859
_cod_original_formula_sum        'Ba1 Co1 O2.23'
_cod_database_code               4124851
Crystal and molecular structure of hexaaquocobalt(II) hexafluorosilicate(IV), (Co (H2 O)6) (Si F6)
Lynton, H.; Siew, P.Y.; Canadian Journal of Chemistry 51 (1973) 227–229; doi:

data_1542050
_publ_section_title
;
 Crystal and molecular structure of hexaaquocobalt(II)
 hexafluorosilicate(IV), (Co (H2 O)6) (Si F6)
;
_journal_name_full               'Canadian Journal of Chemistry'
_journal_page_first              227
_journal_page_last               229
_journal_volume                  51
_journal_year                    1973
_chemical_formula_sum            'Co F6 H12 O6 Si'
_chemical_name_systematic        '(Co (H2 O)6) (Si F6)'
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   9.358
_cell_length_b                   9.358
_cell_length_c                   9.712
_cell_volume                     736.555
_citation_journal_id_ASTM        CJCHAG
_cod_data_source_file            Lynton_CJCHAG_1973_1082.cif
_cod_data_source_block           H12Co1F6O6Si1
_cod_original_cell_volume        736.5553
_cod_original_formula_sum        'H12 Co1 F6 O6 Si1'
_cod_database_code               1542050
Die Struktur von Rhodizit
Strunz, H.; Naturwissenschaften 31 (1943) 68–68; doi:

data_1542051
_publ_section_title
;
 Die Struktur von Rhodizit
;
_journal_name_full               Naturwissenschaften
_journal_page_first              68
_journal_page_last               68
_journal_volume                  31
_journal_year                    1943
_chemical_formula_sum            'Al4 B9.9996 Be2.0004 K Li4 Na O27'
_chemical_name_systematic        'Li4 Na K Al4 Be3 B10 O27'
_space_group_IT_number           215
_symmetry_space_group_name_Hall  'P -4 2 3'
_symmetry_space_group_name_H-M   'P -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   7.3
_cell_length_b                   7.3
_cell_length_c                   7.3
_cell_volume                     389.017
_citation_journal_id_ASTM        NATWAY
_cod_data_source_file            Strunz_NATWAY_1943_1156.cif
_cod_data_source_block           Al4B9.9996Be2.0004K1Li4Na1O27
_cod_original_formula_sum        'Al4 B9.9996 Be2.0004 K1 Li4 Na1 O27'
_cod_database_code               1542051
The Crystal Structures of Mo S2 Cl3 and Mo3 S7 Cl4
Marcoll, J.; Mootz, D.; Rabenau, A.; Wunderlich, H.; Revue de Chimie Minerale 11 (1974) 607–615; doi:

data_1542052
_publ_section_title
;
 The Crystal Structures of Mo S2 Cl3 and Mo3 S7 Cl4
;
_journal_name_full               'Revue de Chimie Minerale'
_journal_page_first              607
_journal_page_last               615
_journal_volume                  11
_journal_year                    1974
_chemical_formula_sum            'Cl4 Mo3 S7'
_chemical_name_systematic        'Mo3 (S2)3 S Cl4'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 122.9
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.336
_cell_length_b                   12.185
_cell_length_c                   13.956
_cell_volume                     1333.000
_citation_journal_id_ASTM        RVCMA8
_cod_data_source_file            Marcoll_RVCMA8_1974_286.cif
_cod_data_source_block           Cl4Mo3S7
_cod_original_cell_volume        1333
_cod_database_code               1542052
Crystal structure of trirubidium hexachlorothallate
Thiele, G.; Richter, R.; Zeitschrift fuer Kristallographie (149,1979-) 205 (1993) 129–130; doi:

data_8104447
_publ_section_title
;
 Crystal structure of trirubidium hexachlorothallate
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              129
_journal_page_last               130
_journal_volume                  205
_journal_year                    1993
_chemical_formula_sum            'Cl6 Rb3 Tl'
_chemical_name_systematic        'Rb3 (Tl Cl6)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 108
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.193
_cell_length_b                   7.964
_cell_length_c                   12.551
_cell_volume                     1254.179
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Thiele_ZEKRDZ_1993_1506.cif
_cod_data_source_block           Cl6Rb3Tl1
_cod_original_formula_sum        'Cl6 Rb3 Tl1'
_cod_database_code               8104447
Structure cristalline du trimetaphosphate de baryum sodium Ba Na P3 O9
Martin, C.; Mitschler, A.; Acta Crystallographica B (24,1968-38,1982) 28 (1972) 2348–2352; doi:

data_2107409
_publ_section_title
;
 Structure cristalline du trimetaphosphate de baryum sodium Ba Na P3 O9
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2348
_journal_page_last               2352
_journal_volume                  28
_journal_year                    1972
_chemical_formula_sum            'Ba Na O9 P3'
_chemical_name_systematic        'Ba Na (P3 O9)'
_space_group_IT_number           19
_symmetry_space_group_name_Hall  'P 2ac 2ab'
_symmetry_space_group_name_H-M   'P 21 21 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.055
_cell_length_b                   12.278
_cell_length_c                   5.785
_cell_volume                     785.217
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Martin_ACBCAR_1972_304.cif
_cod_data_source_block           Ba1Na1O9P3
_cod_original_cell_volume        785.2171
_cod_original_formula_sum        'Ba1 Na1 O9 P3'
_cod_database_code               2107409
Crystal structure of Na, Ca triorthosilicate, Na2 Ca3 (Si3 O10)
Treushnikov, E.N.; Ilyukhin, V.V.; Belov, N.V.; Kristallografiya 16 (1971) 76–79; doi:

data_1542053
_publ_section_title
;
 Crystal structure of Na, Ca triorthosilicate, Na2 Ca3 (Si3 O10)
;
_journal_name_full               Kristallografiya
_journal_page_first              76
_journal_page_last               79
_journal_volume                  16
_journal_year                    1971
_chemical_formula_sum            'Ca3 Na2 O10 Si3'
_chemical_name_systematic        'Na2 Ca3 (Si3 O10)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 93
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   16.38
_cell_length_b                   5.16
_cell_length_c                   11.74
_cell_volume                     990.914
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Treushnikov_KRISAJ_1971_208.cif
_cod_data_source_block           Ca3Na2O10Si3
_cod_original_cell_volume        990.9142
_cod_database_code               1542053
Refinement of the structures of high-calcium monoclinic pyroxenes
Maslenikov, A.V.; Rozhdestvenskaya, I.V.; Zaitsev, V.N.; Kristallografiya 23 (1978) 266–273; doi:

data_1542054
_publ_section_title
;
 Refinement of the structures of high-calcium monoclinic pyroxenes
;
_journal_name_full               Kristallografiya
_journal_page_first              266
_journal_page_last               273
_journal_volume                  23
_journal_year                    1978
_chemical_formula_sum            'Al0.14 Ca0.92 Fe0.41 Mg0.53 O6 Si2'
_chemical_name_systematic        'Ca.92 Fe.08 Al.14 Fe.33 Mg.53 Si2 O6'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 106.11
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.737
_cell_length_b                   8.898
_cell_length_c                   5.27
_cell_volume                     438.662
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Maslenikov_KRISAJ_1978_790.cif
_cod_data_source_block           Al0.14Ca0.92Fe0.41Mg0.53O6Si2
_cod_original_cell_volume        438.6619
_cod_database_code               1542054
The crystal structure of suolunite
Tseng, J.K.; Hsueh, C.Y.; Peng, C.C.; Kexue Tongbao (= Bulletin der Wissenschaften) 17 (1966) 45–48; doi:

data_1542055
_publ_section_title
;
 The crystal structure of suolunite
;
_journal_name_full
'Kexue Tongbao (= Bulletin der Wissenschaften)'
_journal_page_first              45
_journal_page_last               48
_journal_volume                  17
_journal_year                    1966
_chemical_formula_sum            'Ca2 H4 O8 Si2'
_chemical_name_systematic        'Ca2 (H2 Si2 O7) (H2 O)'
_space_group_IT_number           43
_symmetry_space_group_name_Hall  'F 2 -2d'
_symmetry_space_group_name_H-M   'F d d 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.02
_cell_length_b                   19.74
_cell_length_c                   6.08
_cell_volume                     1322.612
_citation_journal_id_ASTM        KETOD8
_cod_data_source_file            Tseng_KETOD8_1966_625.cif
_cod_data_source_block           H4Ca2O8Si2
_cod_original_formula_sum        'H4 Ca2 O8 Si2'
_cod_database_code               1542055
Refinement of the structures of high-calcium monoclinic pyroxenes
Maslenikova, A.V.; Zaitsev, V.N.; Rozhdestvenskaya, I.V.; Kristallografiya 23 (1978) 266–273; doi:

data_1542056
_publ_section_title
;
 Refinement of the structures of high-calcium monoclinic pyroxenes
;
_journal_name_full               Kristallografiya
_journal_page_first              266
_journal_page_last               273
_journal_volume                  23
_journal_year                    1978
_chemical_formula_sum            'Al0.06 Ca0.79 Fe0.68 Mg0.47 O6 Si2'
_chemical_name_systematic        'Ca.79 Al.06 Fe.08 Mg.47 Fe.60 Si2 O6'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.7
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.766
_cell_length_b                   8.598
_cell_length_c                   5.246
_cell_volume                     424.062
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Maslenikova_KRISAJ_1978_791.cif
_cod_data_source_block           Al0.06Ca0.79Fe0.68Mg0.47O6Si2
_cod_original_cell_volume        424.0623
_cod_database_code               1542056
Crystal Structure of Cesium Chlorotrifluoroantimonate
Udovenko, A.A.; Volkova, L.M.; Davidovich, R.L.; Zemnukhova, L.A.; Koordinatsionnaya Khimiya (= Coordination Chemistry (USSR)) 3 (1977) 259–261; doi:

data_1542057
_publ_section_title
;
 Crystal Structure of Cesium Chlorotrifluoroantimonate
;
_journal_name_full
;
Koordinatsionnaya Khimiya (= Coordination Chemistry (USSR))
;
_journal_page_first              259
_journal_page_last               261
_journal_volume                  3
_journal_year                    1977
_chemical_formula_sum            'Cl Cs F3 Sb'
_chemical_name_systematic        'Cs Sb Cl F3'
_space_group_IT_number           121
_symmetry_space_group_name_Hall  'I -4 2'
_symmetry_space_group_name_H-M   'I -4 2 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   9.94
_cell_length_b                   9.94
_cell_length_c                   11.61
_cell_volume                     1147.110
_citation_journal_id_ASTM        KOKHDC
_cod_data_source_file            Udovenko_KOKHDC_1977_583.cif
_cod_data_source_block           Cl1Cs1F3Sb1
_cod_original_cell_volume        1147.11
_cod_original_formula_sum        'Cl1 Cs1 F3 Sb1'
_cod_database_code               1542057
The crystal structure of potassium dithorium trisphosphate, K Th2 (P O4)3
Matkovic, B.; Prodic, B.; Sljukic, M.; Documenta Chemica Yugoslavica. Croatica Chemica Acta 40 (1968) 147–161; doi:

data_1542058
_publ_section_title
;
 The crystal structure of potassium dithorium trisphosphate, K Th2 (P O4)3
;
_journal_name_full
'Documenta Chemica Yugoslavica. Croatica Chemica Acta'
_journal_page_first              147
_journal_page_last               161
_journal_volume                  40
_journal_year                    1968
_chemical_formula_sum            'K O12 P3 Th2'
_chemical_name_systematic        'K Th2 (P O4)3'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 101.77
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   17.57
_cell_length_b                   6.863
_cell_length_c                   8.138
_cell_volume                     960.671
_citation_journal_id_ASTM        CCACAA
_cod_data_source_file            Matkovic_CCACAA_1968_1721.cif
_cod_data_source_block           K1O12P3Th2
_cod_original_cell_volume        960.6711
_cod_original_formula_sum        'K1 O12 P3 Th2'
_cod_database_code               1542058
Crystal structure of europium barium copper aluminium oxide
Usov, O.A.; Kartenko, N.F.; Sapozhnikova, L.S.; Rozhdestvenskaya, I.V.; Zeitschrift fuer Kristallographie (149,1979-) 205 (1993) 285–286; doi:

data_8104448
_publ_section_title
;
 Crystal structure of europium barium copper aluminium oxide
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              285
_journal_page_last               286
_journal_volume                  205
_journal_year                    1993
_chemical_formula_sum            'Al0.419 Ba2 Cu2.581 Eu O6.729'
_chemical_name_systematic        'Eu Ba2 Cu2 (Cu0.581 Al0.419 O6.729)'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.899
_cell_length_b                   3.899
_cell_length_c                   11.707
_cell_volume                     177.972
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Usov_ZEKRDZ_1993_1498.cif
_cod_data_source_block           Al0.419Ba2Cu2.581Eu1O6.729
_cod_original_cell_volume        177.9722
_cod_original_formula_sum        'Al0.419 Ba2 Cu2.581 Eu1 O6.729'
_cod_database_code               8104448
Na2 (Pr4 O2) Cl9, the first reduced quaternary praseodymium chloride with anti-SiS2 analogous Pr4/2-chains
Mattfeld, H.; Meyer, G.; Zeitschrift fuer Anorganische und Allgemeine Chemie 620 (1994) 85–89; doi:

data_1542059
_publ_section_title
;
 Na2 (Pr4 O2) Cl9, the first reduced quaternary praseodymium chloride with
 anti-SiS2 analogous Pr4/2-chains
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              85
_journal_page_last               89
_journal_volume                  620
_journal_year                    1994
_chemical_formula_sum            'Cl9 Na2 O2 Pr4'
_chemical_name_systematic        'Na2 Pr4 Cl9 O2'
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 106.51
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.122
_cell_length_b                   11.341
_cell_length_c                   9.376
_cell_volume                     828.031
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Mattfeld_ZAACAB_1994_1549.cif
_cod_data_source_block           Cl9Na2O2Pr4
_cod_original_cell_volume        828.0307
_cod_database_code               1542059
The crystal structure of Mn (H2 P O4)2 (H2 O)2
Vasic, P.; Prelesnik, B.; Curic, M.; Herak, R.; Zeitschrift fuer Kristallographie (149,1979-) 173 (1985) 193–198; doi:

data_8104449
_publ_section_title
;
 The crystal structure of Mn (H2 P O4)2 (H2 O)2
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              193
_journal_page_last               198
_journal_volume                  173
_journal_year                    1985
_chemical_formula_sum            'H8 Mn O10 P2'
_chemical_name_systematic        'Mn (H2 P O4)2 (H2 O)2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 94.79
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.3774
_cell_length_b                   10.17
_cell_length_c                   7.315
_cell_volume                     398.647
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Vasic_ZEKRDZ_1985_1356.cif
_cod_data_source_block           H8Mn1O10P2
_cod_original_cell_volume        398.6467
_cod_original_sg_symbol_Hall     '-P 2ybc (x-z,y,z)'
_cod_original_formula_sum        'H8 Mn1 O10 P2'
_cod_database_code               8104449